# 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

• Published on
04-Jun-2018

• View
213

0

Embed Size (px)

Transcript

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

1/9

Technical Bulletin September, 2009

3Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

Introduction 3M VHB Tapes have been used worldwide in a variety of applications in the

construction industry since the introduction of these tapes in 1980. To further support

consideration for structural glazing applications, structural performance tests were

conducted at an independent 3rd party test facility (Facade Engineering & Weather

Performance of Buildings Materials Science & Engineering CSIRO, Australia, report

No. DTF 865) toevaluate 3M VHB Structural Glazing Tape under stresses thatglass panels wouldtypically experience in a glazed curtain wall system or commercial windows.

Background Calculation of the width of adhesive bond (Structural Bite Width) required for a

structurally glazed panel is commonly determined by application of Trapezoidal Load

Distribution Theory. This is based on the assumption that rather than remaining flat, a

rectangular panel under wind load will deflect in a tributary area fashion. The tensile

stress on the structural bond around the perimeter varies, with the peak stress occurring at

the center of the longest span:

(1)

The calculation for determining the required Structural Bite Width of bonding material to

resist the peak wind load stress (Design Pressure) is given by the following calculation:

Structural Bite Width (mm) = 1/2 x L x Design Pressure (kPa)Bonding Material Design Stress

Structural Bite Width (in) = 1/2 x L (ft) x Design Pressure (psf)

Bonding Material Design Stress x 12 in/ft

85 kPa (12 psi) is used as the Bonding Material Design Stress derived by dividing the

ultimate tensile failure stress by a safety factor of 5, providing an industry appropriate

margin of safety.

Y

T

Figure 1 - Trapezoidal Model for load Distribution

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

2/9

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(2)

Background(continued)

As negative pressure from a suction wind load is applied to glass panels in a curtain wall

system, secondary shear forces on the bond may result due to the deflection that occurs in

the frame members, in particular the mullions. The material design strength of 3M

VHB Structural Glazing Tape has been well established and in common use in

construction applications for 3M VHB Tapes. The aim of the tests described in this

bulletin is to provide further support for the use of 85kPa (12 psi) as the BondingMaterial Design Stress in a trapezoidal structural bite width calculation. Furthermore, the

tests are designed to validate the calculated Structural Bite Width is also suitable for

accommodating secondary shear forces that occur on 3M VHB Structural Glazing

Tape in glazing systems.

Conclusions 3M VHB Structural Glazing Tape B23F fulfilled all the requirements in the tests

conducted as specified by AS4284 test methods. Furthermore, testing of 3M VHB

Structural Glazing Tape B23F was taken beyond the requirements of AS4284:2008 to

include proof tests at 2x, 3x and 4.15x the design guideline for 3M VHB Structural

Glazing Tapes, demonstrating no evidence of collapse or tape distress. The results of thetests validate the use of 85 kPa (12 psi) as the material design strength in calculation of

the Structural Bite Width in a trapezoidal model calculation, and the test demonstrated at

least a 4x safety factor in this design.

Written assessment of use of the trapezoidal approximation for bite width calculation and

secondary forces based on the test results by the supervising consulting engineer can be

summarized as follows:

1. For most glass panel aspect ratios approximately 2:1, the use of 85 kpa (12 psi)

as the material design strength in a trapezoidal approximation is conservative.

As the aspect ratio approaches 1:1, the use of the trapezoidal approximation

yields structural bite widths up to 5% less than classical plate theory, however

the 5% error is well compensated for with the use of a 5x safety factor in thematerial design strength of 3M VHB Structural Glazing Tape.

2. The shear stress in the tape due to mullion bending (secondary forces) for the

test specimen was calculated at 12.8 kN/m when the test pressure was -2.9 kPa

(-60 psf). This can be compared with other cases for example, using the same

mullion/glass type in a floor-to-floor configuration, 3.9 m (12.75 ft) high (floor

to soffit) with mullions spaced at 1.2m (3.9 ft), using a Serviceability Limit

State design pressure of Pz = 1.0 kPa, then the maximum shear in 7mm (0.28

in) wide tape (as per Trapezoidal Model calculation of Structural Bite) is

9.2kN/m, which is less than the shear in the test tape of 12.8 kN/m at 2.8kPa.

Therefore, the tape has been tested with a shear well in excess of 9.2kN/m

without distress, and will therefore be satisfactory for typical curtainwallsituations.

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

3/9

Test Procedure A sequence of tests were designed and conducted on a test specimen representative for

an actual project using 3M VHB Structural Glazing Tape the structural glazing of

insulated glass unit (double glazed) clerestory windows in the National Portrait Gallery,

Canberra, Australia (Figure 2).

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(3)

Figure 2 Actual arrangement an orientation of Clerestory Window Glazing National

Portrait Gallery

Figure 3 Test Chamber setup & panel

orientation Portrait Gallery

In order to adequately observe the effects of mullion

bending, a three panel part facade test specimen wasconstructed using the same frame members and glass

type. The test specimen was installed into the test

chamber with a 90 rotation compared to the orientation

of the glazing in the National Portrait Gallery in order to

fit into the test chamber (Figure 3).

The wind load design pressure of the panels for the

actual building was -1.66 kPa (-35 psf) for the 1765 mm

(70 in) L x 2400 mm (95 in) W insulated glass unit panels

-10.38 mm (0.41 in) laminated external, 12 mm (0.5 in)

air space, 8 mm (0.31 in) annealed internal. This panel

size and wind load would normally require at least 18 mm(0.71 in) width 3M VHB Structural Glazing Tape as

the structural bite. However, in order to ensure that the

properties of the tape were adequately tested without the

limitation of glass panel or frame failure, the structural

bite width in the test specimen was scaled down to 10 mm

(0.4 in) width 3M VHBStructural Glazing Tape

B23F. This resulted in a design wind load for the 3M

VHB Structural Glazing Tape bond of -0.96 kPa

(-20 psf) while maintaining a design wind load of

-1.66kPa (-35 psf) for the glass & frame.

Structural performance tests were conducted according toAS4284:2008. Additionally, proof tests at 2x, 3x and

4.15x the structural load were conducted and each held

for one minute. Deflections at 22 points on the tests

specimen were measured in order to assess the secondary

forces applied to the glass frame bond.

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

4/9

3 2

1

5

1

4

Test Specimen Set-up

Figure 4 Test Window Frame Elevation

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(4)

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

5/9

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(5)

Figure 5 Mullion detail

1

Spacer

blocks

providing

support

IGU Glass Type:

10.38 mm laminated external, 12 mm

air space, 8 mm annealed internal

2 mm Aluminum

Extrusion Frame

(Powder-coated)

3M VHB Structural Glazing Tape B23F

10 mm (0.4 in) width

2.3 mm (0.090 in) thick

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

6/9

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(6)

Figure 6 Head & Sill detail

3

2

3M VHB Structural Glazing Tape B23F

10 mm (0.4 in) width

Plywood cover over

remaining test chamber

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

7/9

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(7)

Figure 7 Jamb Detail

3M VHB Structural Glazing Tape B23F

10 mm (0.4 in) width

4

5

Timber

block

support

Ground

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

8/9

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(8)

Summary of Results

The following table summarizes the results of the structural performance & proof load tests.

Table 1 Results of Structural Load

Test Method Parameter Results

Structural Performance Test AS4284:2008 +0.96 kPa & -0.96 kPa Pass(Pressure profile as per figure 5) (+20 psf & - 20 psf)

Figure 7 AS4284:2008 Structural Performance Test Pressure Sequence

Table 2 - Results of proof load tests

Test Pressure % of Design Load for 3M VHBTest Method kPa (psf) Structural Glazing Tape Results

Proof Load Tests AS4284:2008 -1.44 (-30) 150% No Collapse

Pressure held for -2.9 (-60) 300%* No Collapse

1 minute at each of -3.3 (-69) 344%* No Collapsethe test pressures -4.0 (-84) 417%* No Collapse

listed

*Not a requirement of AS 4284:2008 or ASTM E330

• 8/13/2019 3M- VHB- Structural Glazing Tapes Structural Performance Tests Technical Bulletin

9/9

Structural Performance & Design Stress ProofTests of 3M VHB Structural Glazing Tape

(9)

All statements, technical information and recommendations contained in this document are based upontests or experience that 3M believes are reliable. However, many factors beyond 3Ms control can affectthe use and performance of a 3M product in a particular application, including the conditions underwhich the product is used and the time and environmental conditions in which the product is expectedto perform. Since these factors are uniquely within the user s knowledge and control, it is essential thatthe user evaluate the 3M product to determine whether it is fit for a particular purpose and suitable forthe users method of application.

Product Use

3M warrants for 24 months from the date of manufacture that 3M VHB Tape will be free of defectsin material and manufacture. 3M MAKES NO OTHER WARRANTIES, EXPRESS OR IMPLIED,INCLUDING BUT NOT LIMITED TO, ANY IMPLIED WARRANTY OF MERCHANTABILITY ORFITNESS FOR A PARTICULAR PURPOSE. This limited warranty does not cover damage resultingfrom the use or inability to use 3M VHB Tape due to misuse, workmanship in application, orapplication or storage not in accordance with 3M recommended procedures. AN APPLICATIONWARRANTY EXPRESSLY APPROVED AND ISSUED BY 3M IS AN EXCEPTION. THE CUSTOMERMUST APPLY FOR A SPECIFIC APPLICATION WARRANTY AND MEET ALL WARRANTY ANDPROCESS REQUIREMENTS TO OBTAIN AN APPLICATION WARRANTY. CONTACT 3M FOR MOREINFORMATION ON APPLICATION WARRANTY TERMS AND CONDITIONS.

Limited Warranty

If the 3M VHB Tape is proved to be defective within the warranty period stated above. THE EXCLUSIVEREMEDY, AT 3MS OPTION, SHALL BE TO REFUND THE PURCHASE PRICE OF OR TO REPAIR ORREPLACE THE DEFECTIVE 3M VHB TAPE. 3M shall not otherwise be liable for loss or damages,whether direct, indirect, special, incidental, or consequential, regardless of the legal theory asserted,including negligence, warranty, or strict liability.

Limitation ofRemedies andLiability

3M and VHB are trademarks of3M Company.

Printed in U.S.A.

3M 2009 70-0709-3991-6 (9/09)

Recycled Paper40% pre-consumer

10% post-consumer

3